Hydrogels for Biomedical Applications: Their Characteristics and the Mechanisms behind Them Qinyuan Chai, Yang Jiao and Xinjun Yu * Department of Chemistry, University of Cincinnati, Cincinnati, OH 45221, USA; [email protected]
(Q.C.); [email protected]
(Y.J.) * Correspondence: [email protected]
; Tel.: +1-513-556-1107 Academic Editor: David Díaz Díaz Received: 16 August 2016; Accepted: 11 January 2017; Published: 24 January 2017
Abstract: Hydrogels are hydrophilic, three-dimensional networks that are able to absorb large quantities of water or biological fluids, and thus have the potential to be used as prime candidates for biosensors, drug delivery vectors, and carriers or matrices for cells in tissue engineering. In this critical review article, advantages of the hydrogels that overcome the limitations from other types of biomaterials will be discussed. Hydrogels, depending on their chemical composition, are responsive to various stimuli including heating, pH, light, and chemicals. Two swelling mechanisms will be discussed to give a detailed understanding of how the structure parameters affect swelling properties, followed by the gelation mechanism and mesh size calculation. Hydrogels prepared from natural materials such as polysaccharides and polypeptides, along with different types of synthetic hydrogels from the recent reported literature, will be discussed in detail. Finally, attention will be given to biomedical applications of different kinds of hydrogels including cell culture, self-healing, and drug delivery. Keywords: hydrogels; biomaterials; drug delivery; self-healing; cell culture
1. Introduction Hydrogels, crosslinked 3D networks of hydrophilic polymer chains, are capable of holding large amounts of water due to their hydrophilic structure [1–4]. Thus, the hydrogel networks can extensively swell in water media. Since water is the greatest component of the human body, a hydrogel, which can absorb large quantities of water, is considered to have great potential when applied for biomedical purposes [5–10]. Recently, wide investigation has been going on into the feasibility of applying hydrogels in fields including tissue engineering, drug delivery, self-healing materials, biosensors, and hemostasis bandages [11–15]. Compared with other types of biomaterials, hydrogels have the advantages of increased biocompatibility, tunable biodegradability, properly mechanical strength, porous structure, and so on. However, due to the low mechanical strength and fragile nature of the hydrogels, the feasibility of applying hydrogels is still limited. Thus, novel hydrogels with stronger and more stable properties are still needed and remain an important direction for research. As expected, naturally formed hydrogels are gradually replaced by synthetic hydrogels to achieve longer service life, high capacity of water absorption, and high gel strength [8,9]. Fortunately, with various developed synthetic strategies, hydrogels with defined network structures, desirable chemical compositions, and tunable mechanical strength can be designed. Hydrogels can be prepared from completely artificial components and show remarkable stability even under severe conditions such as high temperature or a very acidic or basic environment. Additionally, by modifying the polymer chains with stimuli-responsive functional groups, the hydrogel properties can be switched by stimuli including heat, light, magnetic fields, chemical agents, and pH [16–20].
Gels 2017, 3, 6; doi:10.3390/gels3010006
Gels 2017, 3, 6
2 of 15
In this critical review, different technologies for preparing hydrogels will be discussed and we will take a closer look at different kinds of stimuli-responsive hydrogels. Detailed swelling mechanisms proposed based on various theories will be covered to give a deeper understanding of such materials. Last but not least, attention will be given to different hydrogels to achieve specific requirements for biomedical purposes such as cell culture, self-healing, and drug delivery. 2. Different Kinds of Stimuli-Responsive Hydrogels Defined by Peppas , “hydrogels are hydrophilic, three-dimension networks, which are able to imbibe large amounts of water or biological fluids, and thus resemble, to a large extent, a biological tissue”. They are insoluble in any solvent due to the polymer chains being crosslinked by either covalent bonds or physical interactions such as entanglements and crystallites [22–24]. Due to the properties of hydrogels, such as high content of water, soft and rubbery consistence, as well as low interfacial tension with water or biological fluids, they are expected to be potential alternatives for natural tissues . According to different applications, the hydrogel can be prepared to respond to various stimuli in the body such as pH, ionic strength, and temperature. 2.1. Thermoresponsive Hydrogels The equilibrium between the hydrophobic and hydrophilic segments is the key to control the properties of a synthetic thermoresponsive hydrogel. In detail, the temperature has a remarkable effect on the hydrophobic interactions between hydrophobic polymer segments and the hydrophilic interactions between hydrophilic polymer segments and water molecules. Thus, a small temperature change can interrupt the original equilibrium and induce sol–gel transition . In the work done by Vernon’s group , they synthesized a temperature-responsive graft copolymer based on N-isopropylacrylamide (NIPAAm) and Jeffamine M-1000 acrylamide (JAAm), which showed controlled swelling properties without introducing degradable moieties or increasing the lower critical solution temperature (LCST) above body temperature. The JAAm was hypothesized to be useful as a component in the polymer architecture to control the swelling and release properties with minimal effect on LCST. The outstanding hydrolytic stability, hydrophilicity, and minimal LCST effect make this hydrogel a suitable candidate for a variety of temperature-responsive biomaterials where control over swelling or drug release is crucial. In another work , Long and co-workers investigated the application of a poly(N-isopropylacrylmide) (PNIPAAm) hydrogel thin film to thermochromic smart windows. The solar modulating ability (∆Tsol ) showed an ultra-large value with the luminous transmittance (Tlum ) to be highest identified so far. This hydrogel demonstrated an excellent combination of high Tlum along with dramatically improved solar modulating ability, which may lead to the development of thermochromic smart windows based on organic materials. 2.2. pH-Responsive Hydrogels pH-Responsive hydrogels are a class of biomaterials that exhibit desirable physical and chemical properties at specific pH ranges. Acidic or basic groups are bonded to the polymer chains. The acidic groups deprotonate at high pH, while the basic groups protonate at low pH. The association, dissociation, and binding of various ions to polymer chains cause hydrogel swelling in an aqueous solution. Peppa’s group fabricated a hydrophilic pH-responsive hydrogel based on poly(methyacrylicgraft-ethylene glycol) (P(MMA-g-EG)) conjugated with hydrophobic PMMA nanoparticles . By incorporating a different mole ratio of PMMA nanoparticles in the P(MMA-g-EG), it forms amphiphilic polymer carriers with tunable physical properties. The release of encapsulated therapeutic agents triggered by a change of pH from the stomach to the small intestine was tested. Furthermore, the cyto-compatibility of the polymer materials was investigated on cells modeling the gastrointestinal
Gels 2017, 3, 6 Gels 2017, 3, 6
3 of 15 3 of 14
P(MMA-g-EG) provides the possibility to be used asnanoparticle oral delivery vectors ofP(MMA-g-EG) chemotherapeutics for (GI) tract and colon cancer cells. This pH-responsive containing provides cancer. the possibility to be used as oral delivery vectors of chemotherapeutics for cancer. In general, general, the the size size of of the In the gel gel will will respond respond to to environment environment pH pH as as well well as as salt salt concentration. concentration. Thus, Thus, an equilibrium equilibrium model model was was established established by by Moore’s Moore’s group group to to predict predictthe the swelling/deswelling swelling/deswelling behavior an behavior of hydrogels of of thethe model was conducted by comparing the of hydrogels in in different differentpH pHsolutions. solutions.The Thevalidation validation model was conducted by comparing simulations with experimental results. This model was then utilized to investigate the effects of the simulations with experimental results. This model was then utilized to investigate the effects of different hydrogels hydrogels and and solution solution conditions conditions on on the the degree degree and andrate rateof ofswelling/deswelling swelling/deswelling of of those those different hydrogels . It was found that the higher the concentration and buffer diffusivity are, the faster the hydrogels . It was found that the higher the concentration and buffer diffusivity are, the faster kinetic. All these parameters can be used to tune the performance of hydrogel microactuators, the kinetic. All these parameters can be used to tune the performance of hydrogel microactuators, suggesting that that the the mechanical mechanical properties properties of of the the hydrogel hydrogel can can be be varied varied considerably considerably by by varying varying the the suggesting pH of solutions. pH of solutions. 2.3. Light- and Chemical-Responsive Hydrogels Light-responsive hydrogels are promising functional materials for potential application in the areas delivery , micro lenses , sensors , etc. due to the fact that the activation areas of of drug/gene drug/gene delivery process via light light can can be be remote remote and and noninvasive. noninvasive. The prepared hydrogel consists of aa deoxycholic deoxycholic acid-modified β-cyclodextrin derivative and and an azobenzen-branched azobenzen-branched poly(acrylic poly(acrylic acid) acid) copolymer, β-cyclodextrin derivative and can be converted efficiently from gel to sol phase upon photo irradiation irradiation with with light light of of 355 355 nm. nm. to gel gel phase phase upon upon photo photo irradiation irradiation with light of 450 nm The hydrogel was able to recover from sol to . The reversible transition (Figure 1) . transition of this hydrogel can be controlled under mild condition, suggesting that that this thisgel gelmaterial materialhas hasaapromising promisingrole roleininbioengineering bioengineering applications release suggesting applications forfor thethe release of of molecular cellular species. molecular andand cellular species.
Figure 1. 1. Supramolecular formed from from deoxycholate-β-CD deoxycholate-β-CD derivative derivative 22 and and Figure Supramolecular inclusion inclusion complex complex 11 formed azobenzene-branched poly(acrylic poly(acrylic acid) copolymer 3.  with with permission permission from from the the azobenzene-branched acid) copolymer 3. Reprinted Reprinted from from  American Chemical Society (2009). American Chemical Society (2009).
In another example, a novel light-responsive hydrogel was made from a poly(NIn another example, a novel light-responsive hydrogel was made from a poly(N-isopropylacrylamide) isopropylacrylamide) (PNIPAAm) nanocomposite incorporating glycidyl methacrylate (PNIPAAm) nanocomposite incorporating glycidyl methacrylate functionalized graphene oxide functionalized graphene oxide (GO-GMA). As a result, the nanocomposite hydrogel will undergo a (GO-GMA). As a result, the nanocomposite hydrogel will undergo a large volume change under large volume change under stimulation of infrared (IR) light, because of the highly efficient photo stimulation of infrared (IR) light, because of the highly efficient photo thermal conversion of GO-GMA. thermal conversion of GO-GMA. This material has the potential to be used as an actuator in This material has the potential to be used as an actuator in microelectromechanical systems or microelectromechanical systems or microfluidic devices . microfluidic devices . In a different work done by Maeda’s group , they reported DNA-responsive hydrogels that In a different work done by Maeda’s group , they reported DNA-responsive hydrogels “only shrunk” by the addition of ssDNA (single-stranded DNA) samples (Figure 2). This biomaterial that “only shrunk” by the addition of ssDNA (single-stranded DNA) samples (Figure 2). was developed by polyacrylamide (polyAAm) hydrogels containing directly grafted ssDNA or an ssDNA-polyAAm conjugate in a semi-interpenetrating network. Unlike traditional stimuliresponsive hydrogels, this conjugate retains the advantage of using cross-linkable ssDNAs with well-
Gels 2017, 3, 6
4 of 15
This biomaterial was developed by polyacrylamide (polyAAm) hydrogels containing directly grafted ssDNA or6 an ssDNA-polyAAm conjugate in a semi-interpenetrating network. Unlike traditional Gels 2017, 3, 4 of 14 stimuli-responsive hydrogels, this conjugate retains the advantage of using cross-linkable ssDNAs characterized conformational properties,properties, thus providing in DNA sensing or with well-characterized conformational thus potential providingapplications potential applications in DNA DNA-triggered actuators. actuators. sensing or DNA-triggered
Figure 2. The The response response of of novel novel hybrid hybrid hydrogels hydrogels containing containing ssDNA ssDNA as as aa cross-linker cross-linker to to ssDNA. ssDNA. Reprinted from  with permission from the American Chemical Society Society (2005). (2005).
3. Mechanism 3. Different Different Theories Theories behind behind the the Hydrogel Hydrogel Swelling Swelling Mechanism The propertiesofofhydrogels hydrogels specific applications depend onbulk theirstructures. bulk structures. For The properties forfor specific applications depend on their For network network characterizations, are important several important parameters as volume fraction structurestructure characterizations, there arethere several parameters such assuch volume fraction in the in the swollen state, the corresponding mesh size, and the molecular weight of the polymer chain swollen state, the corresponding mesh size, and the molecular weight of the polymer chain between between neighboring points. Thefraction volumeoffraction of polymers in thestate swollen state is a neighboring crosslink crosslink points. The volume polymers in the swollen is a parameter parameter describing how much fluid can be absorbed and retained. The molecular weight between describing how much fluid can be absorbed and retained. The molecular weight between neighboring neighboring crosslink points, either covalent bond or physical interaction, is a parameter describing crosslink points, either covalent bond or physical interaction, is a parameter describing the degree the degree of crosslinking. These are parameters related and cantheoretically be calculated of crosslinking. These parameters related toare each other to andeach can other be calculated or theoretically or determined by a variety of experimental techniques. In the following paragraph, the determined by a variety of experimental techniques. In the following paragraph, the two most widely two widely used methods,swelling the equilibrium swelling theoryelasticity and the rubber theory, will usedmost methods, the equilibrium theory and the rubber theory, elasticity will be discussed. be discussed. 3.1. Equilibrium Swelling Theory 3.1. Equilibrium Swelling Theory The Flory–Rehner equation describes the mixing of polymers and liquid molecules, which can be Flory–Rehner equation the mixing of polymers andstatus liquidofmolecules, which can usedThe to analyze hydrogels withoutdescribes ionic domains . The equilibrium the hydrogel swollen be used to analyze hydrogels without ionic domains . The equilibrium status of the hydrogel in a fluid is determined by two reverse forces. One is the thermodynmical force of mixing favors swollen a fluid determined by two reverse Onepolymer is the thermodynmical of mixing swelling,inwhile theisother is the stored force in theforces. stretched chains hinderingforce swelling . favors swelling, while balance the otherout is the in the stretched polymer chains hindering swelling These two forces eachstored otherforce as described in Equation (1) for the physical situation in . terms of the Gibbs free energy: These two forces balance out each other as described in Equation (1) for the physical situation in ∆Gtotal = ∆Gelastic + ∆Gmixing (1) terms of the Gibbs free energy: ∆Gstored total = ∆G elastic + mixing where ∆Gelastic comes from the elastic forces in∆G the extended polymer chains contained(1)in the gelΔG networks; ∆Gfrom is the result fromforces the mixing molecules the polymer mixing the where elastic comes elastic stored in thebetween extendedfluid polymer chainswith contained in the chains. The mixing factor is result a measure the compatibility the polymer with the solvent molecules, gel networks; ΔGmixing is the fromofthe mixing betweenoffluid molecules with the polymer chains. which is usually by the polymer–solvent interaction parameter, . molecules, which The mixing factorexpressed is a measure of the compatibility of the polymer with theχsolvent is usually expressed by the polymer–solvent interaction parameter, χ . Differentiation of Equation (1) with respect to the number of solvent molecules, while keeping the temperature and pressure constant, gives Equation (2): µ1 - µ1,o = ∆µelastic + ∆µmixing .
Gels 2017, 3, 6
5 of 15
Differentiation of Equation (1) with respect to the number of solvent molecules, while keeping the temperature and pressure constant, gives Equation (2): µ1 − µ1,o = ∆µelastic + ∆µmixing .
In the equilibrium status, the chemical potential outside the gel should be equal to the chemical potential inside the gel (∆µ1,o = ∆µ1 ). As a result, the chemical potential change from free energy of mixing and elastic force stored in the stretched polymer chains have to cancel out each other. The previous Flory–Rehner theory was modified for a hydrogel synthesized from aqueous phase. The water contained sufficiently changed chemical potential due to elastic forces, which is responsible for the change of volume fraction density of the polymer chains in the crosslinking process . The presence of ionic moieties in hydrogel makes the situation much more complex, due to thermo complex system from the ionic domain of the polymer chains, which introduces an extra changing factor into the Gibbs free energy. 3.2. Rubber Elasticity Theory From a mechanical perspective, hydrogels assemble natural rubbers that deform elastically in response to applied stress. Treloar  and Flory  utilized the elastic properties of the hydrogels to describe their structure. However, the original elasticity theory does not apply to hydrogels prepared in solvent. The theory of rubber elasticity by Peppas as in Equation (3)  is the only form used to analyze the hydrogel structure, with hydrogels prepared in solvent: v2,s 1/3 2Mc 1 $RT 1 − α − 2 τ = , v2,r α Mc Mn
where τ is the applied stress to the polymer sample, $ is the density of the polymer, R is the universal gas constant, T is the absolute experimental temperature, and Mc is the molecular weight between crosslinks. To utilize this elasticity theory to analyze the structure of the hydrogel, experiments must be done in the tensile mode [43,44]. 3.3. Mechanism of Gelation In the thermally induced sol–gel transition, there are different processes involved including hydrophobic and hydrophilic interactions, coil to helix transition, micelle packing, and so on. To understand the exact gelation mechanism behind certain polymers, figuring out the exact molecular level process is essential . The most widely reported thermally induced gelation is based on the equilibrium between hydrophobic and hydrophilic interactions. For example, introducing a hydrophobic segment such as methyl, ethyl, or propyl to hydrophilic polymers is an efficient way to tune the hydrophobicity of the polymer . LCST is a critical temperature below which the system will be miscible and above which phase separation will occur, forming gels. Interactions between polymer and polymer, polymer and water, and water and water take place in aqueous polymer solutions. The LCST of the system depends on the equilibrium status of these interactions. The most efficient way to determine LCST is by light scattering, with the collapse and aggregation of the polymer chains during gelation state inducing a dramatic increase of the light scattering . Thermodynamically, the thermally induced abrupt change in the solubility is controlled by the Gibbs free energy of mixing . A small change in temperature can cause negative change in the Gibbs free energy. As a result, the interaction between polymer and water will be eliminated and the water–water and polymer–polymer interaction will be favored. To equilibrate this negative Gibbs free energy change, there must be an increase in the entropy term due to the already known increased enthalpy term. Due to the dramatic increase in the hydrophobic interactions between polymer chains, at the sol–gel transition temperature, the polymer chains quickly dehydrate and collapse to a more hydrophobic structure [45,49]. On the other hand, some amphiphilic block copolymers will
Gels 2017, 3, 6
6 of 15
self-assemble into micelle structures due to the hydrophobic interaction to equilibrate the decrease of the Gibbs free energy . Depending on the concentration, amphiphilic block copolymers can form micelles, which are aggregates of surfactant molecules dispersed in a liquid colloid and hydrogels by adding water and adjusting the temperature. These block copolymers build up a structure with a hydrophobic core and hydrophilic shell with typical micelle size between 20 and 100 nm. All the gelation mechanisms discussed here are based on reversible physical linkage, so the gelation transition is reversible after removing the gelling stimuli. 3.4. Calculation of the Mesh Size The space contained in a hydrogel, responsible for the diffusion properties, is often regarded as the ‘pore’. Depending on the size of these pores, hydrogels are commonly classified as macro-pores, micro-porous, or non-porous. The size of the pore is often described by a structural parameter, the correlation length ξ, which is defined as the linear distance between two neighboring crosslinks : 1/2 ξ = α ro 2 .
Here, α is the elongation ratio of the polymer chains and r o stands for the distance between two adjacent crosslinking points of the unperturbed polymer chain . From the volume fraction of the swollen polymer v2,s , the elongation ratio α can be calculated as: −1/3 α = v2,s .
The unperturbed end-to-end distance of the polymer chain between two neighboring crosslinks can be calculated by: 1/2 ro 2 = l (C n N )1/2 , (6) where l is the length of the bond along the polymer backbone (1.54 Å for vinyl polymers), Cn is the Flory characteristic ratio, and N, the number of links per chain, can be calculated by: N =
2Mc , Mr
where Mr is the molecular weight of the repeat unit. Finally, combining all the equations above, the correlated distance of the polymer chains between two adjacent crosslinking points can be evaluated: ξ =
2Cn Mc Mr
4. Hydrogels Based on Natural Materials 4.1. Hydrogels Based on Polysaccharides Cellulose is a natural polysaccharide that cannot dissolve in water. Unlike other types of water-soluble polysaccharides, cellulose requires separate cross-linking to fabricate a hydrogel network . Native cellulose nanofibers are normally generated from bacterial and plants. Those nanofibers prefer to disperse in an aqueous solution rather than dissolving . In Yliperttula and co-workers’ work , a plant-derived nanofibrillar cellulose (NFC) hydrogel with desired functionality makes a potential 3D cell culture scaffold. The structural properties of NFC hydrogel were evaluated along with rheological properties, cellular biocompatibility, cellular polarization, and differentiation of human hepatic cell lines. Due to its fluid-like property, NFC was demonstrated to
Gels 2017, 3, 6
7 of 15
be injectable at high stress, which makes it possible to mix into gels. Furthermore, spontaneous gelation after injection imparted the necessary mechanical support for both cell growth and differentiation. Another technique was developed to immobilize an enzyme/antibody. After partial oxidation by sodium periodate, a cellulose hydrogel was prepared from an aqueous alkali-urea solvent. This enabled the cellulose gel to further introduce aldehyde groups . By a Schiff base formation between the aldehyde and amino groups of protein, various active proteins can be covalently introduced to a cellulose gel and stabilized by a reduction of imines, which was confirmed by a coloring reaction. The same strategy is applicable to the peroxidase antibody, which makes various active proteins have the ability to be immobilized on cellulose gels by mild and facile processing. Due to the excellent chemical and mechanical stability of cellulose, this strategy and the afforded materials have the potential to be used for biochemical processing and sensing materials. Reported by Lee and co-workers , by the use of a biocompatible ionic liquid, lipase from Candida rugosa was successfully trapped into various cellulose–biopolymer composite hydrogels. A biocompatible ionic liquid, 1-ethyl-3-methylimidazolium acetate, was used, which is known to be one of the best solvents for lignocellulosic materials among the ionic liquids (ILs). The lipase was successfully immobilized in various cellulose composite hydrogels, which is the first report that successfully entrapped an enzyme into non-derivatized cellulose–biopolymer composite hydrogels. 4.2. Hydrogels Based on Polypeptides Gelatin is a denatured product of collagen, a mixture of peptides and proteins produced by partial hydrolysis of collagen extracted from the skin, bones, and connective tissues of animals, which is easily available, degradable, and demonstrates good biocompatibility in vivo. Also, gelatin retains cell-binding motifs such as arginylglycylaspartic acid (RGD) and matrix metalloproteinase (MMP)-sensitive degradation sites, which is the critical component in cell encapsulation [58,59]. Kao’s group  developed an easy strategy using cysteine to modify gelatin through a bifunctional PEG. In this way, free thio groups can be introduced to gelatin chains based on thiolated gelatin and poly(ethylene glycol) diacrylate. Varying concentration and ratio of precursor provides these crosslinked gelatin-based hydrogels with easy mechanical property modulation. In a 3D environment, gelatin crosslinking modality is crucial for long-term integrin binding sites as well as supporting cell attachment and proliferation by cell morphology and proliferation study. In another study done by Melero-Martin’s group , they demonstrated that bioengineering human vascular networks inside methacrylated gelatin (GelMA) constructed in a liquid form could be injected into immunodeficient mice, followed by instantaneous crosslinking when exposed to UV light. A solution of GelMA containing human blood-derived endothelial colony-forming cells (ECFCs) and bone marrow-derived mesenchymal stem cells (MSCs) can be injected into the subcutaneous space of an immunodeficient mouse and then rapidly crosslinked with a controllable degree of GelMA through the exposure time to UV light. For future regenerative applications, which require the formation of functional vascular beds in vivo, GelMA is a good way to deliver vascular cells due to its injectable form before crosslinking. In another example , a three-dimensional scaffold containing self-assembled polycaprolactone (PCL) sandwiched in a gelatin-chitosan hydrogel was developed for application as a biodegradable patch for surgical reconstruction of congenital heart defects; it contains a thin, self-assembled PCL core, intended to facilitate handling, cutting, and suturing the material and to provide sufficient tensile strength to function in the ventricular wall. The developed novel hydrogel was demonstrated to have significant potential to be used as a cardiac patch that can repair congenital cardiac defects. 5. Synthetic Hydrogels Synthetic polymer-based hydrogels, due to their widely variable and easily tuned properties, have been extensively studied. By varying the chemical composition and preparation methods, the structure of the hydrogels can be controlled. Beneficial properties including porosity, swelling
Gels 2017, 3, 6
8 of 15
ability, stability, biocompatibility/biodegradability, and mechanical strength can all be tuned for specific application purposes. For example, vehicles with a controlled release rate for either small molecular or macromolecular drugs including DNA, enzymes, and peptides can be achieved . Filipovic’s group  synthesized a novel temperature-and pH-sensitive hydrogel based on N-isopropylacrylamide (NIPAAm) and itaconic acid (IA) through free radical polymerization with lipase extracted from Candida rugosa, which is a promising system that can be applied as a pH-responsive device for drug delivery purposes. The properties of these prepared hydrogels were found to be highly sensitive to changes of temperature and pH, while keeping the ionic strength constant. A series of hydrogels was prepared with different molar ratios of NIPAAm and IA. Their morphology, mechanical properties, swelling degree, protein loading efficiency, and release rate were all evaluated. The protein release pattern clearly depends on the extent of swelling of the hydrogels. Vuluga and co-workers reported the synthesis of a novel thermoresponsive crosslinked hydrogel based on different molecular weight of poly(propylene glycol)s (PPG) and diepoxy-terminated poly(ethylene glycol)s (PEG) to control the multi-block copolymer structure . In an ideal situation, the hydrogel structure is expected to contain one PPG block and two PEG chains linked to the same amine group, leading to a structure with each PPG block surrounded by four PEG blocks, while each PEG block has two PPG blocks and two PEG blocks as neighbors. Both thermoresponsive and swelling properties can be adjusted by controlling the molecular weight of the constituent blocks or the salt added in. For synthetic hydrogels, in addition to single network hydrogels, hydrogels consisting of two independently crosslinked polymer networks attracted wide attention recently, for which tough gels can be formed even with a less crosslinked “second work” within a more highly crosslinked “first network”. The molar ratio of the second network repeat units to the first network needs to be >5 . In the work done by Spinks’s group , a novel double network hydrogel was synthesized with a bottlebrush structure formed from oligo-monomers of poly(ethylene glycol) methyl ether methacrylate as the first polymer network and poly(acrylic acid) as the second network. The strong intermolecular interactions between the neutral poly(ethylene glycol) side chains and the non-ionic groups offer the hydrogel excellent mechanical strength and high sensitivity to pH changes. Such a material with robust nature and sensitivity to pH changes has a potential as artificial muscles or controlled release devices. In situ gelable interpenetrating double-network hydrogels have been formulated, prepared from thiolated chitosan and oxidized dextran in a one-pot process. No potentially cytotoxic small-molecule cross-linkers are required and they are without complex maneuvers or catalysis. It was reported that the interpenetrating double-network structure enhanced the mechanical properties and gelation performance of the hydrogel formulated from the thiolated chitosan. In conclusion, this hydrogel system is promising as an in situ formable biomaterial for clinically related applications requiring mechanical strength, durability, and fast gelation . A new inorganic–organic double-network hydrogel composing of poly(acrylic acid) and graphene was prepared with the as-prepared 3D graphene architecture to be the first network and acrylic acid monomer dispersed into the consecutive channels and polymerized which is the second network. This inorganic–organic double-network hydrogel shows both flexibility and electrical conductivity, and can be used in the next generation of flexible electric devices . 6. Applications in Biomedical Field 6.1. Hydrogels for Three-Dimensional Cell Culture Hydrogels, with high water content as well as tissue-like mechanical properties, have been demonstrated to be capable of combining with cells to engineer various tissues in both vitro and vivo [69,70]. A crucial requirement for the construction of three-dimensional regenerative tissue in sufficient quantities is an artificially created environment that enables biological cells to grow or interact
Gels 2017, 3, 6
9 of 15
with their surroundings in all three dimensions. Anseth’s group  reported a new cross-linking chemistry by the tetrazine-norbornene click reaction for the formation of cell-laden hydrogels for 3D cell culture (Figure 3). A PEG functionalized with benzylamino tetrazine moiety was specifically chosen and used Gels 2017, 3, 6because in their previous work it was shown to have high reactivity toward norbornene. 9 of 14 The bio-orthogonality, ideal reaction kinetics, and amenability to photochemical patterning made this hydrogel have applications in a progression variety of fundamental well as also translational alternativeplatform to improve thepotential understanding of disease on a cellularas level and to screen tissue engineering applications. anti-cancer drugs.
Figure 3. 3. Synthetically formed using using Figure Synthetically tractable tractable click click hydrogels hydrogels for for three-dimensional three-dimensional cell cell culture culture formed tetrazine–norbornene chemistry. with permission permission from from the the American American Chemical Chemical tetrazine–norbornene chemistry. Reprinted Reprinted from from   with Society (2013). Society (2013).
6.2. Hydrogels for Self-Healing Another work was done by Loessner and co-workers . They characterized gelatin Self-healing(GelMA)-based is one of the most outstanding properties of natural materials such spheroid-based as skin, bones, methacrylamide hydrogels and established them as in vitro and in vivo and wood. Thus, hydrogels that can self-heal open up another field for biomedical applications models for ovarian cancer, to efficiently reflect the advanced disease stage of patients. Hydrogels of [73,74].size, Even though and synthetic hydrogels are were fabricated to mimic biological tissues, mostpreparation of the time equal diffusion, physical properties generated by employing a controlled they validation still lack the ability toSuch self-heal. This drawback will limit theirasutilization in many applications and protocol. GelMA-based hydrogels served a low-cost, reproducible, and that require highforstress. As acell consequence, researchers a as lotanofalternative effort to improving tailorable matrix 3D cancer cultures. Thus, they can dedicate be applied to improve the the mechanical properties of hydrogels, the self-healing property. understanding of disease progressionincluding on a cellular level and also to screen anti-cancer drugs. The process of healing cracks in natural systems usually contains an energy dissipation 6.2. Hydrogels for Self-Healing mechanism. The self-healing can occur in the presence of sacrificial bonds, which can break and reform dynamically before or during the failure occurring. preparematerials a self-healing both Self-healing is one of the most outstanding properties To of natural such hydrogel, as skin, bones, covalent [75,76] and non-covalent [77,78] interactions have been reported. and wood. Thus, hydrogels that can self-heal open up another field for biomedical applications [73,74]. synthesis of novel hydrogels containing reversible oxime tissues, crosslinks were reported by EvenThe though synthetic hydrogels are fabricated to mimic biological most of the time they Mukherjee ; they are capable of autonomous healing as a consequence of their dynamic nature. still lack the ability to self-heal. This drawback will limit their utilization in many applications that To prepare copolymers containing ketoafunctional were synthesized by require high these stress.hydrogels, As a consequence, researchers dedicate lot of effortgroups to improving the mechanical copolymerizing N,N-dimethylacrylamide (DMA) and diacetone acrylamide (DAA) via free radical properties of hydrogels, including the self-healing property. polymerization. Then thecracks afforded hydrophilic copolymers were covalently crosslinked with The process of healing in natural systems usually contains an energy dissipation mechanism. difunctional alkoxyamine obtain hydrogels by thebonds, formation oxime. with dynamically the efficient The self-healing can occur intothe presence of sacrificial whichofcan breakAlong and reform self-healing ability, the reversibility of oxime linkages also led to reversible gel-to-sol transitions before or during the failure occurring. To prepare a self-healing hydrogel, both covalent [75,76] and when excess monofunctional alkoxyamine was added at ambient temperature. non-covalent [77,78] interactions have been reported. Othersynthesis than chemical cross-linkers, interactionsoxime can also play an important role asby a The of novel hydrogelshydrophobic containing reversible crosslinks were reported cross-linker for self-healing hydrogels. Okay’s group developed a hydrogel by copolymerization of Mukherjee ; they are capable of autonomous healing as a consequence of their dynamic nature. a large hydrophobic monomer stearyl methacrylate andfunctional dococyl acrylate with synthesized a hydrophilic To prepare these hydrogels, copolymers containing keto groups were by monomer acrylamide in a micellar solution(DMA) of sodium sulfate . After the addition of salt, copolymerizing N,N-dimethylacrylamide anddodecyl diacetone acrylamide (DAA) via free radical micelles grow andThen solubilize hydrophobes. This hydrogel was demonstrated to have a high degree polymerization. the afforded hydrophilic copolymers were covalently crosslinked with of toughness due to the finite lifetime of hydrophobic interactions between stearyl methacrylate and difunctional alkoxyamine to obtain hydrogels by the formation of oxime. Along with the efficient dococyl acrylate blocks. self-healing ability, the reversibility of oxime linkages also led to reversible gel-to-sol transitions when A monofunctional different work alkoxyamine was recently was reported and co-workers . In this research, excess addedby at Yamauchi ambient temperature. hydrogels containing cationic substituents were prepared via free-radical polymerization. After applying an aqueous dispersion of Micaromica to the surface, when brought into contact the hydrogels adhered strongly due to the intercalation of cationic substituents included in the gel networks into the interlayers of Micromica. The adhesive strength became higher and was able to support a tensile load of 10 kg as the water content ratio of hydrogels decreased (Figure 4).
Gels 2017, 3, 6
10 of 15
Other than chemical cross-linkers, hydrophobic interactions can also play an important role as a cross-linker for self-healing hydrogels. Okay’s group developed a hydrogel by copolymerization of a large hydrophobic monomer stearyl methacrylate and dococyl acrylate with a hydrophilic monomer acrylamide in a micellar solution of sodium dodecyl sulfate . After the addition of salt, micelles grow and solubilize hydrophobes. This hydrogel was demonstrated to have a high degree of toughness due to the finite lifetime of hydrophobic interactions between stearyl methacrylate and dococyl acrylate blocks. A different work was recently reported by Yamauchi and co-workers . In this research, hydrogels containing cationic substituents were prepared via free-radical polymerization. After applying an aqueous dispersion of Micaromica to the surface, when brought into contact the hydrogels adhered strongly due to the intercalation of cationic substituents included in the gel networks into the interlayers of Micromica. The adhesive strength became higher and was able to support a tensile load of 10 kg3,as6 the water content ratio of hydrogels decreased (Figure 4). Gels 2017, 10 of 14
Figure Figure 4. 4. Schematic Schematicrepresentation representationofofhigh highconcentration concentrationcationic cationicgels gelsadhered adheredusing using 1.6 1.6 mg mg of of Micromica supporting a tensile load of 10 kg. Reprinted from  with permission from the American Micromica supporting a tensile load of 10 kg. Reprinted from  with permission from the American Chemical ChemicalSociety Society(2016). (2016).
6.3. 6.3.Hydrogels Hydrogelsfor forDrug DrugDelivery Delivery To deliver drugs, drugs,porous porousstructure structure hydrogels provide a matrix for loading drug loading and To deliver of of hydrogels cancan provide a matrix for drug and protect protect drugs from hostile environment at the same time. Moreover, this porosity can be controlled drugs from hostile environment at the same time. Moreover, this porosity can be controlled by varying by the crosslinking of the gel matrix. The release rate,important another important parameter thevarying crosslinking density of density the gel matrix. The release rate, another parameter for drug for drug carriers, mainly depends on the diffusion coefficient of this molecule through the and gel carriers, mainly depends on the diffusion coefficient of this molecule through the gel network network and can also be tuned according to specific requirements. Biocompatibility and can also be tuned according to specific requirements. Biocompatibility and biodegradability can be biodegradability can be obtained by and designing chemical and physical structures for obtained by designing certain chemical physicalcertain structures for hydrogels. All of those properties hydrogels. All of those properties lend hydrogels great potential to be used for drug delivery [46,82]. lend hydrogels great potential to be used for drug delivery [46,82]. Poly Poly (ethylene (ethylene oxide)-b-poly(propylene oxide)-b-poly(propylene oxide)-b-poly oxide)-b-poly (ethylene (ethylene oxide) oxide) triblock triblock copolymers copolymers (PEO–PPO–PEO) (PEO–PPO–PEO)(known (knownas asPluronic Pluronicor or Poloxamer) Poloxamer)have have been been extensively extensively used used in in pharmaceutical pharmaceutical systems systems. . Paavola Paavolaand andco-workers co-workersfabricated fabricatedan aninjectable injectablegel gelbased basedon onPoloxamer Poloxamerto tocarry carry and and control the release of the anesthetic agent lidocaine . Since Poloxamer is commercially available, control the release of the anesthetic agent lidocaine . Since Poloxamer is commercially available, this hospital utilization. utilization. Nevertheless, this method method was was proven proven to to be be suitable suitable for for hospital Nevertheless, the the relatively relatively rapid rapid diffusion of drugs out of the gel matrix, as well as the duration of drug release, is still diffusion of drugs out of the gel matrix, as well as the duration of drug release, is still limited. limited. ItItcan can be improved by covalent crosslinking with other functional group, such as ethoxysilane, amine, be improved by covalent crosslinking with other functional group, such as ethoxysilane, amine,or or carbohydrates, carbohydrates,to toprevent prevent the the dilution dilution of of the the polymer polymer in in water water [85–87]. [85–87]. In Inaddition, addition,to toload loaddrug druginto intoaagel gelmatrix, matrix,conjugating conjugatingdrugs drugsto toaahydrogel hydrogelcrosslinked crosslinkednetwork network isis another anotherway way to to deliver deliver drugs. drugs. Zhu Zhu and and co-workers co-workersreported reportedaa supramolecular supramolecularbased basedhydrogel hydrogelto to deliver (DOX).First, First,they theysynthesized synthesized a supramolecular polymeric prodrug via host– deliver doxorubicin doxorubicin (DOX). a supramolecular polymeric prodrug via host–guest guest interaction between cyclodextrin-functionalized polyaldehyde and DOX-modified adamantine. After crosslinking by carboxymethyl chitosan, an injectable DOX-loaded hydrogel was created. This hydrogel was shown to release DOX when exposed to acid stimuli . 7. Conclusions
Gels 2017, 3, 6
11 of 15
interaction between cyclodextrin-functionalized polyaldehyde and DOX-modified adamantine. After crosslinking by carboxymethyl chitosan, an injectable DOX-loaded hydrogel was created. This hydrogel was shown to release DOX when exposed to acid stimuli . 7. Conclusions Compared with other types of biomaterials, hydrogels have distinct properties such as high water content, controllable swelling behavior, ease of handing, as well as biocompatibility, which makes them attractive for biomedical applications. Based on their chemical structure and crosslink network, hydrogels can respond to different types of stimuli including thermal, pH, light, and chemical stimuli, which can meet various application requirements. Two different hydrogel swelling mechanisms were discussed to give a thorough understanding of how the bulky structure affects the properties of the swollen hydrogels under specific conditions. Hydrogels based on natural materials such as polysaccharides and polypeptides, along with synthetic hydrogels were exampled in detail. Hydrogels, which are three-dimensional crosslinked polymeric networks able to swell in large amounts of water, should be considered prime candidates for carriers or matrices for cells in tissue engineering, self-healing materials, and delivery vehicles for drugs and biomolecules. Further research should be directed to achieving high mechanical strength, fast and efficient self-healing ability, and various biological activities for different biomedical purposes. Author Contributions: Qinyuan Chai, Yang Jiao and Xinjun Yu contributed equally to this work. Conflicts of Interest: The authors declare no conflict of interest.
References 1. 2. 3. 4. 5.
6. 7. 8. 9. 10. 11.
Ahmed, E.M. Hydrogel: Preparation, characterization, and applications: A review. J. Adv. Res. 2015, 6, 105–121. [CrossRef] [PubMed] Sun, Y.; Kaplan, J.A.; Shieh, A.; Sun, H.-L.; Croce, C.M.; Grinstaff, M.W.; Parquette, J.R. Self-assembly of a 5-fluorouracil-dipeptide hydrogel. Chem. Commun. 2016, 52, 5254–5257. [CrossRef] [PubMed] Kim, S.H.; Sun, Y.; Kaplan, J.A.; Grinstaff, M.W.; Parquette, J.R. Photo-crosslinking of a self-assembled coumarin-dipeptide hydrogel. New J. Chem. 2015, 39, 3225–3228. [CrossRef] Verhulsel, M.; Vignes, M.; Descroix, S.; Malaquin, L.; Vignjevic, D.M.; Viovy, J.L. A review of microfabrication and hydrogel engineering for micro-organs on chips. Biomaterials 2014, 35, 1816–1832. [CrossRef] [PubMed] Daniele, M.A.; Adams, A.A.; Naciri, J.; North, S.H.; Ligler, F.S. Interpenetrating networks based on gelatin methacrylamide and PEG formed using concurrent thiol click chemistries for hydrogel tissue engineering scaffolds. Biomaterials 2014, 35, 1845–1856. [CrossRef] [PubMed] Yu, X.; Jiao, Y.; Chai, Q. Applications of Gold Nanoparticles in Biosensors. Nano LIFE 2016, 6, 1642001. [CrossRef] Yu, X.; Chen, X.; Chai, Q.; Ayres, N. Synthesis of polymer organogelators using hydrogen bonding as physical cross-links. Colloid Polym. Sci. 2016, 294, 59–68. [CrossRef] Billiet, T.; Vandenhaute, M.; Schelfhout, J.; van Vlierberghe, S.; Dubruel, P. A review of trends and limitations in hydrogel-rapid prototyping for tissue engineering. Biomaterials 2012, 33, 6020–6041. [CrossRef] [PubMed] Hoffman, A.S. Hydrogels for biomedical applications. Adv. Drug Deliv. Rev. 2012, 64, 18–23. [CrossRef] Wang, T.; Jiao, Y.; Chai, Q.; Yu, X. Gold Nanoparticles: Synthesis and Biological Applications. Nano LIFE 2015, 5, 1542007. [CrossRef] Ding, R.; Yu, X.; Wang, P.; Zhang, J.; Zhou, Y.; Cao, X.; Tang, H.; Ayres, N.; Zhang, P. Hybrid photosensitizer based on amphiphilic block copolymer stabilized silver nanoparticles for highly efficient photodynamic inactivation of bacteria. RSC Adv. 2016, 6, 20392–20398. [CrossRef] Lee, K.Y.; Mooney, D.J. Hydrogels for tissue engineering. Chem. Rev. 2001, 101, 1869–1880. [CrossRef] [PubMed] Pan, L.; Yu, G.; Zhai, D.; Lee, H.R.; Zhao, W.; Liu, N.; Wang, H.; Tee, B.C.K.; Shi, Y.; Cui, Y.; et al. Hierarchical nanostructured conducting polymer hydrogel with high electrochemical activity. Proc. Natl. Acad. Sci. USA 2012, 109, 9287–9292. [CrossRef] [PubMed]
Gels 2017, 3, 6
14. 15. 16.
20. 21. 22.
23. 24. 25. 26. 27. 28.
31. 32. 33. 34. 35. 36.
12 of 15
Zhai, D.; Liu, B.; Shi, Y.; Pan, L.; Wang, Y.; Li, W.; Zhang, R.; Yu, G. Highly sensitive glucose sensor based on Pt nanoparticle/polyaniline hydrogel heterostructures. ACS Nano 2013, 7, 3540–3546. [CrossRef] [PubMed] Li, L.; Wang, Y.; Pan, L.; Shi, Y.; Cheng, W.; Shi, Y.; Yu, G. A nanostructured conductive hydrogels-based biosensor platform for human metabolite detection. Nano Lett. 2015, 15, 1146–1151. [CrossRef] [PubMed] Zhu, Z.; Guan, Z.; Jia, S.; Lei, Z.; Lin, S.; Zhang, H.; Ma, Y.; Tian, Z.Q.; Yang, C.J. [email protected]
nanoparticle encapsulated target-responsive hydrogel with volumetric bar-chart chip readout for quantitative point-of-care testing. Angew. Chem. Int. Ed. 2014, 53, 12503–12507. Pan, G.; Guo, Q.; Ma, Y.; Yang, H.; Li, B. Thermo-responsive hydrogel layers imprinted with RGDS peptide: A system for harvesting cell sheets. Angew. Chem. Int. Ed. 2013, 52, 6907–6911. [CrossRef] [PubMed] Yu, X.; Cao, X.; Chen, X.; Ayres, N.; Zhang, P. Triplet–triplet annihilation upconversion from rationally designed polymeric emitters with tunable inter-chromophore distances. Chem. Commun. 2015, 51, 588–591. [CrossRef] [PubMed] Koetting, M.C.; Guido, J.F.; Gupta, M.; Zhang, A.; Peppas, N.A. pH-responsive and enzymatically-responsive hydrogel microparticles for the oral delivery of therapeutic proteins: Effects of protein size, crosslinking density, and hydrogel degradation on protein delivery. J. Control. Release 2016, 221, 18–25. [CrossRef] [PubMed] Jin, Z.; Liu, X.; Duan, S.; Yu, X.; Huang, Y.; Hayat, T.; Li, J. The adsorption of Eu(III) on carbonaceous nanofibers: Batch experiments and modeling study. J. Mol. Liq. 2016, 222, 456–462. [CrossRef] Peppas, N.A.; Merrill, E.W. Poly(vinyl alcohol) hydrogels: Reinforcement of radiation-crosslinked networks by crystallization. J. Polym. Sci. A Polym. Chem. 1976, 14, 441–457. [CrossRef] Matanovi´c, M.R.; Kristl, J.; Grabnar, P.A. Thermoresponsive polymers: Insights into decisive hydrogel characteristics, mechanisms of gelation, and promising biomedical applications. Int. J. Pharm. 2014, 472, 262–275. [CrossRef] [PubMed] Peppas, N. Hydrogels of poly(vinyl alcohol) and its copolymers. Hydrogels Med. Pharm. 1986, 2, 1–48. Peppas, N.A.; Mongia, N.K. Ultrapure poly(vinyl alcohol) hydrogels with mucoadhesive drug delivery characteristics. Eur. J. Pharm. Biopharm. 1997, 43, 51–58. [CrossRef] Hamidi, M.; Azadi, A.; Rafiei, P. Hydrogel nanoparticles in drug delivery. Adv. Drug Deliv. Rev. 2008, 60, 1638–1649. [CrossRef] [PubMed] Bajpai, A.K.; Shukla, S.K.; Bhanu, S.; Kankane, S. Responsive polymers in controlled drug delivery. Prog. Polym. Sci. 2008, 33, 1088–1118. [CrossRef] Overstreet, D.J.; McLemore, R.Y.; Doan, B.D.; Farag, A.; Vernon, B.L. Temperature-responsive graft copolymer hydrogels for controlled swelling and drug delivery. Soft Matter 2013, 11, 294–304. [CrossRef] Zhou, Y.; Cai, Y.; Hu, X.; Long, Y. Temperature-responsive hydrogel with ultra-large solar modulation and high luminous transmission for “smart window” applications. J. Mater. Chem. A 2014, 2, 13550–13555. [CrossRef] Schoener, C.A.; Hutson, H.N.; Peppas, N.A. pH-responsive hydrogels with dispersed hydrophobic nanoparticles for the oral delivery of chemotherapeutics. J. Biomed. Mater. Res. A 2013, 101, 2229–2236. [CrossRef] [PubMed] De, S.K.; Aluru, N.; Johnson, B.; Crone, W.; Beebe, D.J.; Moore, J. Equilibrium swelling and kinetics of pH-responsive hydrogels: Models, experiments, and simulations. J. Microelectromech. Syst. 2002, 11, 544–555. [CrossRef] Jeong, B.; Bae, Y.H.; Lee, D.S.; Kim, S.W. Biodegradable block copolymers as injectable drug-delivery systems. Nature 1997, 388, 860–862. [PubMed] Dong, L.; Jiang, H. Autonomous microfluidics with stimuli-responsive hydrogels. Soft Matter 2007, 3, 1223–1230. [CrossRef] Holtz, J.H.; Asher, S.A. Polymerized colloidal crystal hydrogel films as intelligent chemical sensing materials. Nature 1997, 389, 829–832. [CrossRef] Zhao, Y.-L.; Stoddart, J.F. Azobenzene-Based Light-Responsive Hydrogel System. Langmuir 2009, 25, 8442–8446. [CrossRef] [PubMed] Lo, C.-W.; Zhu, D.; Jiang, H. An infrared-light responsive graphene-oxide incorporated poly(N-isopropylacrylamide) hydrogel nanocomposite. Soft Matter 2011, 7, 5604–5609. [CrossRef] Murakami, Y.; Maeda, M. DNA-responsive hydrogels that can shrink or swell. Biomacromolecules 2005, 6, 2927–2929. [CrossRef] [PubMed]
Gels 2017, 3, 6
37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47.
48. 49. 50.
51. 52. 53. 54. 55.
56. 57. 58. 59. 60. 61.
13 of 15
Flory, P.J.; Rehner, J., Jr. Statistical mechanics of cross-linked polymer networks II. Swelling. J. Chem. Phys. 1943, 11, 521–526. [CrossRef] Flory, P.J. Principles of Polymer Chemistry; Cornell University Press: Ithaca, NY, USA, 1953. Peppas, N.A.; Merrill, E.W. Crosslinked poly(vinyl alcohol) hydrogels as swollen elastic networks. J. Appl. Polym. Sci. 1977, 21, 1763–1770. [CrossRef] Treloar, L.R.G. The Physics of Rubber Elasticity; Oxford University Press: Oxford, UK, 1975. Flory, P.J.; Rabjohn, N.; Shaffer, M.C. Dependence of elastic properties of vulcanized rubber on the degree of cross linking. J. Polym. Sci. 1949, 4, 225–245. [CrossRef] Peppas, N.; Bures, P.; Leobandung, W.; Ichikawa, H. Hydrogels in pharmaceutical formulations. Eur. J. Pharm. Biopharm. 2000, 50, 27–46. [CrossRef] Lowman, A.M.; Peppas, N.A. Analysis of the complexation/decomplexation phenomena in graft copolymer networks. Macromolecules 1997, 30, 4959–4965. [CrossRef] Mark, J.E. Polymer Networks; Springer: Heidelberg, Germany, 1982; pp. 1–26. Klouda, L.; Mikos, A.G. Thermoresponsive hydrogels in biomedical applications. Eur. J. Pharm. Biopharm. 2008, 68, 34–45. [CrossRef] [PubMed] Qiu, Y.; Park, K. Environment-sensitive hydrogels for drug delivery. Adv Drug Deliver Rev. 2001, 53, 321–339. [CrossRef] Gao, X.; Cao, Y.; Song, X.; Zhang, Z.; Xiao, C.; He, C.; Chen, X. pH-and thermo-responsive poly(N-isopropylacrylamide-co-acrylic acid derivative) copolymers and hydrogels with LCST dependent on pH and alkyl side groups. J. Mater. Chem. B 2013, 1, 5578–5587. [CrossRef] Schild, H. Poly(N-isopropylacrylamide): Experiment, theory and application. Prog. Polym. Sci. 1992, 17, 163–249. [CrossRef] Ruel-Gariépy, E.; Leroux, J.-C. In situ-forming hydrogels—Review of temperature-sensitive systems. Eur. J. Pharm. Biopharm. 2004, 58, 409–426. [CrossRef] [PubMed] Mortensen, K.; Pedersen, J.S. Structural study on the micelle formation of poly(ethylene oxide)-poly (propylene oxide)-poly (ethylene oxide) triblock copolymer in aqueous solution. Macromolecules 1993, 26, 805–812. [CrossRef] Jaeger, J.A. Landscape division, splitting index, and effective mesh size: New measures of landscape fragmentation. Landsc. Ecol. 2000, 15, 115–130. [CrossRef] Canal, T.; Peppas, N.A. Correlation between mesh size and equilibrium degree of swelling of polymeric networks. J. Biomed. Mater. Res. 1989, 23, 1183–1193. [CrossRef] [PubMed] Cheng, Y.; Luo, X.; Payne, G.F.; Rubloff, G.W. Biofabrication: Programmable assembly of polysaccharide hydrogels in microfluidics as biocompatible scaffolds. J. Mater. Chem. 2012, 22, 7659–7666. [CrossRef] Klemm, D.; Kramer, F.; Moritz, S.; Lindström, T.; Ankerfors, M.; Gray, D.; Dorris, A. Nanocelluloses: A New Family of Nature-Based Materials. Angew. Chem. Int. Ed. 2011, 50, 5438–5466. [CrossRef] [PubMed] Bhattacharya, M.; Malinen, M.M.; Lauren, P.; Lou, Y.-R.; Kuisma, S.W.; Kanninen, L.; Lille, M.; Corlu, A.; GuGuen-Guillouzo, C.; Ikkala, O. Nanofibrillar cellulose hydrogel promotes three-dimensional liver cell culture. J. Control. Release 2012, 164, 291–298. [CrossRef] [PubMed] Isobe, N.; Lee, D.-S.; Kwon, Y.-J.; Kimura, S.; Kuga, S.; Wada, M.; Kim, U.-J. Immobilization of protein on cellulose hydrogel. Cellulose 2011, 18, 1251–1256. [CrossRef] Kim, M.H.; An, S.; Won, K.; Kim, H.J.; Lee, S.H. Entrapment of enzymes into cellulose–biopolymer composite hydrogel beads using biocompatible ionic liquid. J. Mol. Catal. B Enzym. 2012, 75, 68–72. [CrossRef] Bott, K.; Upton, Z.; Schrobback, K.; Ehrbar, M.; Hubbell, J.A.; Lutolf, M.P.; Rizzi, S.C. The effect of matrix characteristics on fibroblast proliferation in 3D gels. Biomaterials 2010, 31, 8454–8464. [CrossRef] [PubMed] Nichol, J.W.; Koshy, S.T.; Bae, H.; Hwang, C.M.; Yamanlar, S.; Khademhosseini, A. Cell-laden microengineered gelatin methacrylate hydrogels. Biomaterials 2010, 31, 5536–5544. [CrossRef] [PubMed] Fu, Y.; Xu, K.; Zheng, X.; Giacomin, A.J.; Mix, A.W.; Kao, W.J. 3D cell entrapment in crosslinked thiolated gelatin-poly(ethylene glycol) diacrylate hydrogels. Biomaterials 2012, 33, 48–58. [CrossRef] [PubMed] Lin, R.-Z.; Chen, Y.-C.; Moreno-Luna, R.; Khademhosseini, A.; Melero-Martin, J.M. Transdermal regulation of vascular network bioengineering using a photopolymerizable methacrylated gelatin hydrogel. Biomaterials 2013, 34, 6785–6796. [CrossRef] [PubMed]
Gels 2017, 3, 6
68. 69. 70. 71.
73. 74. 75.
79. 80. 81.
14 of 15
Pok, S.; Myers, J.D.; Madihally, S.V.; Jacot, J.G. A multilayered scaffold of a chitosan and gelatin hydrogel supported by a PCL core for cardiac tissue engineering. Acta Biomater. 2013, 9, 5630–5642. [CrossRef] [PubMed] Milašinovi´c, N.; Kalagasidis Kruši´c, M.; Kneževi´c-Jugovi´c, Z.; Filipovi´c, J. Hydrogels of N-isopropylacrylamide copolymers with controlled release of a model protein. Int. J. Pharm. 2010, 383, 53–61. [CrossRef] [PubMed] Anghelache, A.; Teodorescu, M.; Sti´c, M.; Kneževi´c-Jugovi´c, Z.; Filipovi´c, J. Novel crosslinked thermoresponsive hydrogels with controlled poly(ethylene glycol)—poly(propylene glycol) multiblock copolymer structure. Colloid Polym. Sci. 2014, 292, 829–838. [CrossRef] Gong, J.P.; Katsuyama, Y.; Kurokawa, T.; Osada, Y. Double-Network Hydrogels with Extremely High Mechanical Strength. Adv. Mater. 2003, 15, 1155–1158. [CrossRef] Naficy, S.; Razal, J.M.; Whitten, P.G.; Wallace, G.G.; Spinks, G.M. A pH-sensitive, strong double-network hydrogel: Poly(ethylene glycol) methyl ether methacrylates–poly(acrylic acid). J. Polym. Sci. B Polym. Phys. 2012, 50, 423–430. [CrossRef] Zhang, H.; Qadeer, A.; Chen, W. In situ gelable interpenetrating double network hydrogel formulated from binary components: Thiolated chitosan and oxidized dextran. Biomacromolecules 2011, 12, 1428–1437. [CrossRef] [PubMed] Huang, P.; Chen, W.; Yan, L. An inorganic–organic double network hydrogel of graphene and polymer. Nanoscale 2013, 5, 6034–6039. [CrossRef] [PubMed] Baroli, B. Hydrogels for tissue engineering and delivery of tissue-inducing substances. J. Pharm. Sci. 2007, 96, 2197–2223. [CrossRef] [PubMed] Nicodemus, G.D.; Bryant, S.J. Cell encapsulation in biodegradable hydrogels for tissue engineering applications. Tissue Eng. B Rev. 2008, 14, 149–165. [CrossRef] [PubMed] Alge, D.L.; Azagarsamy, M.A.; Donohue, D.F.; Anseth, K.S. Synthetically tractable click hydrogels for three-dimensional cell culture formed using tetrazine–norbornene chemistry. Biomacromolecules 2013, 14, 949–953. [CrossRef] [PubMed] Kaemmerer, E.; Melchels, F.P.; Holzapfel, B.M.; Meckel, T.; Hutmacher, D.W.; Loessner, D. Gelatine methacrylamide-based hydrogels: An alternative three-dimensional cancer cell culture system. Acta Biomater. 2014, 10, 2551–2562. [CrossRef] [PubMed] Wu, D.Y.; Meure, S.; Solomon, D. Self-healing polymeric materials: A review of recent developments. Prog. Polym. Sci. 2008, 33, 479–522. [CrossRef] Thakur, V.K.; Kessler, M.R. Self-healing polymer nanocomposite materials: A review. Polymer 2015, 69, 369–383. [CrossRef] Deng, G.; Li, F.; Yu, H.; Liu, F.; Liu, C.; Sun, W.; Jiang, H.; Chen, Y. Dynamic hydrogels with an environmental adaptive self-healing ability and dual responsive sol–gel transitions. ACS Macro Lett. 2012, 1, 275–279. [CrossRef] Amiri, S.; Rahimi, A. Hybrid nanocomposite coating by sol–gel method: A review. Iran Polym. J. 2016, 25, 559–577. [CrossRef] Bode, S.; Bose, R.; Matthes, S.; Ehrhardt, M.; Seifert, A.; Schacher, F.; Paulus, R.; Stumpf, S.; Sandmann, B.; Vitz, J. Self-healing metallopolymers based on cadmium bis(terpyridine) complex containing polymer networks. Polym. Chem. 2013, 4, 4966–4973. [CrossRef] Burattini, S.; Colquhoun, H.M.; Fox, J.D.; Friedmann, D.; Greenland, B.W.; Harris, P.J.; Hayes, W.; Mackay, M.E.; Rowan, S.J. A Self-repairing, supramolecular polymer system: Healability as a consequence of donor–acceptor π–π stacking interactions. Chem. Commun. 2009, 6717–6719. [CrossRef] [PubMed] Mukherjee, S.; Hill, M.R.; Sumerlin, B.S. Self-healing hydrogels containing reversible oxime crosslinks. Soft Matter 2015, 11, 6152–6161. [CrossRef] [PubMed] Tuncaboylu, D.C.; Sari, M.; Oppermann, W.; Okay, O. Tough and self-healing hydrogels formed via hydrophobic interactions. Macromolecules 2011, 44, 4997–5005. [CrossRef] Tamesue, S.; Yasuda, K.; Noguchi, S.; Mitsumata, T.; Yamauchi, T. Highly Tolerant and Durable Adhesion between Hydrogels Utilizing Intercalation of Cationic Substituents into Layered Inorganic Compounds. ACS Macro Lett. 2016, 5, 704–708. [CrossRef] Gupta, P.; Vermani, K.; Garg, S. Hydrogels: From controlled release to pH-responsive drug delivery. Drug Discov. Today 2002, 7, 569–579. [CrossRef]
Gels 2017, 3, 6
85. 86. 87. 88.
15 of 15
Hoare, T.R.; Kohane, D.S. Hydrogels in drug delivery: Progress and challenges. Polymer 2008, 49, 1993–2007. [CrossRef] Paavola, A.; Yliruusi, J.; Kajimoto, Y.; Kalso, E.; Wahlström, T.; Rosenberg, P. Controlled release of lidocaine from injectable gels and efficacy in rat sciatic nerve block. Pharm. Res. 1995, 12, 1997–2002. [CrossRef] [PubMed] Sosnik, A.; Cohn, D. Ethoxysilane-capped PEO–PPO–PEO triblocks: A new family of reverse thermo-responsive polymers. Biomaterials 2004, 25, 2851–2858. [CrossRef] [PubMed] Cho, K.Y.; Chung, T.W.; Kim, B.C.; Kim, M.K.; Lee, J.H.; Wee, W.R.; Cho, C.S. Release of ciprofloxacin from poloxamer-graft-hyaluronic acid hydrogels in vitro. Int. J. Pharm. 2003, 260, 83–91. [CrossRef] Kim, M.R.; Park, T.G. Temperature-responsive and degradable hyaluronic acid/Pluronic composite hydrogels for controlled release of human growth hormone. J. Control. Release 2002, 80, 69–77. [CrossRef] Xiong, L.; Luo, Q.; Wang, Y.; Li, X.; Shen, Z.; Zhu, W. An injectable drug-loaded hydrogel based on a supramolecular polymeric prodrug. Chem. Commun. 2015, 51, 14644–14647. [CrossRef] [PubMed] © 2017 by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).